- Nano Express
- Open Access
Optical Modulation of the Diffraction Efficiency in an Indoline Azobenzene/Amorphous Polycarbonate Film
© The Author(s). 2016
Received: 16 February 2016
Accepted: 5 July 2016
Published: 15 July 2016
We have made a diffraction grating in an indoline azobenzene/amorphous polycarbonate film by two-beam interference at 532 nm that periodically photodegrades the indoline azobenzene dye. Subsequent illumination of the film with 532-nm light into the trans-isomer band leads to trans-cis isomerization in the indoline azobenzene dye and results in a decrease in the trans-isomer band absorption coefficient. This causes the diffraction efficiency to decrease when probed at 655 nm. The diffraction efficiency returns to its original value when the 532-nm light is blocked by thermal relaxation from the indoline azobenzene cis-isomer to the trans-isomer. Thus, we have been able to optically modulate the diffraction efficiency in a thin film diffraction grating.
Optical filters based on diffraction gratings have a large range of applications that include optical storage [1, 2], optical communication [3–5], strain and chemical sensing [6–9], and spectroscopy [10–12]. They have been made and researched using different methods and materials. For example, doped photorefractive LiNbO3 single crystals have been used to make optical filters where they are made permanent by thermal fixing [3, 13]. Optical filters have also been produced using liquid crystals [14–16], porous silicon [9, 12], anodic aluminina , polymers [4, 18], photochromic films [19, 20], nonlinear optical chromophore thin films , and RbCdF3:Mn2+ single crystals . Optically switchable diffraction gratings would be particularly useful for all-optical switching and multiplexing  and could be used, for example, in add/drop  modules in optical communication systems that are needed for dense wavelength division multiplexing.
We have recently shown that an optically switchable diffraction grating can be made using a photochromic dye/amorphous polycarbonate (APC) composite film. In that case, the dye used was 5-chloro-1,3-dihydro-1,3,3-trimethylspiro[2H-indole-2,3′-(3H)naphth[2,1-b](1,4)oxazine] where UV light is required to break a band that results in a visible absorption band . It was shown that a diffraction grating could be made by two-beam interference, the grating could subsequently be turned on by UV irradiation, and it could disappear after the UV light is turned off. This method does require the use of UV light to turn the diffraction grating on, and it would be advantageous if another dye is used that only requires more easily accessible visible or infrared light.
In this paper, we report the results from optical measurements on a film containing an indoline azobenzene dye in an APC matrix where a two-beam interference method was used to create a diffraction grating. We show that a diffraction grating can be made and the diffraction efficiency can be reduced by exposure to visible light and the recovery of the grating occurs by thermal relaxation.
A photochromic dye/polymer thin film was made using APC and an indoline azobenzene (IAB) dye. The APC used was APEC 9389, and it was obtained from Bayer Materials Science. IAB was synthesized via coupling of the diazonium salt of 4-aminobenzonitrile to 1,3,3-trimethyl-2-methylene indoline using standard conditions. The product was obtained as a red solid, and it was purified by recrystallization in ethanol. An IAB/APC thin film was prepared that contained 5 % of IAB by weight. This was done by dissolving 50 mg of the dye and 950 mg of APC in 10 mL of 1,1,2-trichloroethane (TCE) and stirring the solution for 30 min at ~40 °C. The solution was then passed through 0.45- and then 0.22-μm syringe filters. The solution was spin-coated onto 25 × 25 mm2 glass substrates to create the thin film that was dried in a vacuum in the dark at 80 °C for several days. To minimize the risk of any unintended photo-switching, the dried films were kept in the dark until required.
An Ocean Optics spectrometer or a PerkinElmer Lambda 1050 spectrophotometer was used to make the optical measurements. The film was 2.6-μm thick as estimated from the resultant thin film interference. The optically induced changes in the IAB absorbance were measured by placing a cuvette containing a IAB/TCE solution in the Ocean Optics spectrometer. An initial absorbance measurement was made, and then the solution was exposed to an expanded 532-nm laser beam from a 5-W diode-pumped solid-state frequency-doubled Nd:YVO4 laser. This was immediately followed by an absorbance measurement. The photo-induced changes in the absorption coefficient from the IAB/APC film at 488 nm were measured using the 488-nm line from an Ar ion laser. The beam was split into two beams, and the probe beam went through a 1 % neutral density filter.
A diffraction grating was made in the IAB/APC film by using a cube beam splitter to split the 532-nm laser beam into two beams that overlapped on the film surface. The first-order diffracted beam from one of the beams was used to monitor the resultant diffraction efficiency. The angle between the beams was 3.2°. The diffraction efficiency was also probed at 655 nm where there is no absorption from the IAB dye using a 10-mW diode laser where the incident intensity was 5 mW. Silicon photodiodes were used to measure the transmitted and diffracted beam intensities.
Results and Discussion
Thermal relaxation can be seen in Fig. 3b when the 488-nm switching laser light was blocked. The 1/e thermal relaxation time was ~116 s. Photodegradation occurs for high intensities, as can be seen in Fig. 3c for a 488-nm switching beam intensity of 38 mW/mm2. The film containing IAB initially switches, and then there is a gradual decrease in the absorption coefficient. The switching beam was blocked after 27,550 s, and it can be seen that the absorption coefficient increased by only 170 cm−1 after this time and it does not increase back to the initial value. This shows that there is photodegradation of IAB.
The photodegradation process during high-intensity 488-nm illumination is likely to be oxygen-mediated and similar to that seen in other organic compounds [26–28]. Optical excitation leads to an excited singlet state, and relaxation occurs via a transition to the singlet ground state as well as intersystem crossing to the triplet ground state that leads to the generation of singlet oxygen [26–28]. The transition from the ground state triplet to the lower energy ground singlet state is spin-forbidden, but it can occur in the presence of triplet oxygen and results in the generation of singlet oxygen. It is the singlet oxygen that chemically interacts with dye and leads to the loss of the visible absorption band. This is a well-known problem in organic dyes, and it can be significantly reduced by encapsulation as well as by using singlet oxygen quenchers [28–31].
We have shown above that photo-induced changes in α can be made in a film containing IAB. For low intensities and times, these changes are nearly reversible and there is minimal photodegradation of IAB. However, there is significant photodegradation for high intensities, which can be exploited to create diffraction gratings as shown below.
The diffraction grating was probed using a 655-nm laser beam at normal incidence after an hour which is much longer than the IAB thermal relaxation time. A diffracted beam was observed that arises from periodic photobleaching of IAB that occurred when the film when exposed to the two 532-nm laser beams used to create the grating. Six hundred fifty-five nanometers was chosen as the probe wavelength because at this wavelength, the IAB absorption coefficient is zero and hence Δα in Eq. 1 is zero. It is therefore possible to estimate Δn from Eq. 1 using the measured first-order diffraction efficiency. We show in Fig. 4b that η 1 = 0.0078 %, and from Eq. 1, we estimate that Δn = 0.0014.
The IAB/APC film was exposed to a single 532-nm laser beam in the trans-isomer absorption band at a small angle from normal incidence with an intensity of 111 μW/mm2 at 61 s and continually probed using the 655-nm laser beam. This caused the diffraction efficiency to decrease to 0.0055 % as can be seen in Fig. 4b. This decrease is due to some trans- to cis-isomerization that leads to a reduction in the trans-isomer absorption coefficient and hence the refractive index at 655 nm. We estimate the resultant Δn from Eq. 1 to be Δn = 0.0012 where we find that it has reduced by 0.0002. The 532-nm laser was blocked after 455 s, and the diffraction efficiency increased back to 0.0078 % by thermal relaxation from the cis to the trans-isomer. Thus, the diffraction efficiency was reduced by ~30 % by illumination at 532 nm. This shows that the trans-cis isomerization process can be used to modulate the diffraction efficiency. Higher 532-nm intensities or lower switching wavelengths are required to further decrease the diffraction efficiency.
In conclusion, we have shown that a diffraction grating can be made in an IAB/APC thin film by two-beam interference and periodic photodegradation of the IAB dye. Illumination at a later time with a single beam at 532 nm into the trans-isomer band that is centered ~470 nm leads to a structural transition to the cis-isomer and a concomitant reduction in the trans-isomer band absorption coefficient. This results in a decrease in the diffraction efficiency when probed at 655 nm. The diffraction grating thermally relaxes back to the original diffraction efficiency when the 532-nm laser beam is blocked. Thus, we have shown that it is possible to optically modulate the diffraction efficiency in a thin film containing a dye that displays trans-cis isomerization.
We acknowledge funding from the New Zealand Ministry of Business, Innovation and Employment (Contracts CO8X0704, CO8X0807, and RTVU1405) and the MacDiarmid Institute for Advanced Materials and Nanotechnology.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Coufal HJ, Psaltis D, Sincerbox GT (2000) Holographic data storage. Springer, BerlinView ArticleGoogle Scholar
- Stronski A, Axhimova E, Paiuk O, Meshalkin A, Abashkin V, Lytvyn O, Sergeev SS, Prisacar A, Triduh G (2016) Holographic and e-Beam image recording in Ge5As37S58–Se nanomultilayer structures. Nanoscale Res Lett 11:39View ArticleGoogle Scholar
- Nee I, Beyer O, Müller M, Buse K (2003) Multichannel wavelength-division multiplexing with thermally fixed Bragg gratings in photorefractive lithium niobate crystals. J Opt Soc Am B 20:1593View ArticleGoogle Scholar
- Alavijeh HK, Baghban MA, Parsanasab GM, Sarailou E, Gharavi A, Javadpour S (2008) Add/drop filter using in-plane slanted gratings in azo polymers. Opt Lett 33:2152View ArticleGoogle Scholar
- Telbiz G, Bugaychuk S, Leonenko E, Derzhypolska L, Gnatovskyy V, Pryafko I (2015) Ability of dynamic holography in self-assembled hybrid nanostructured silica films for all-optical switching and multiplexing. Nanoscale Res Lett 10:196View ArticleGoogle Scholar
- O’Dwyer MJ, Ye CC, James SW, Tatam RP (2004) Thermal dependence of the strain response of optical fibre Bragg gratings. Meas Sci Technol 15:1607View ArticleGoogle Scholar
- Rao YJ (1999) Recent progress in applications of in-fibre Bragg grating sensors. Optics and Lasers in Engineering 31:297View ArticleGoogle Scholar
- Stephens KJ, Williams GVM, Monfils I, Hirst D, Wagner P, Raymond SG, Quilty JW (2011) Optics-based strain sensing system. Materials Science Forum 700:178View ArticleGoogle Scholar
- Lai M, Sridharan GM, Parish G, Bhattacharya S, Keating A (2012) Multilayer porous silicon diffraction gratings operating in the infrared. Nanoscale Res Lett 7:645View ArticleGoogle Scholar
- Barbastathis G, Balberg M, Brady DJ (1999) Confocal microscopy with a volume holographic filter. Opt Lett 24:811View ArticleGoogle Scholar
- Psaltis D (2002) Coherent optical information systems. Science 298:1359View ArticleGoogle Scholar
- Mescheder U, Khazi I, Kovacs A, Ivanov A (2014) Tunable optical filters with wide wavelength range based on porous multilayers. Nanoscale Res Lett 9:427View ArticleGoogle Scholar
- Jerez VA, de Oliveira I, Frejlich J (2009) Fixed photorefractive holograms with maximum index-of-refraction modulation in LiNbO3:Fe. J Appl Phys 106:063116View ArticleGoogle Scholar
- Bunning TJ, Natarajan LV, Tondiglia VP, Sutherland RL (2000) Holographic polymere-dispersed liquid crystals (H-PDLCs). Annu Rev Mater Sci 30:83View ArticleGoogle Scholar
- Ono H, Takahashi F, Emoto A, Kawatsuki N (2005) Polarization holograms in azo dye-doped polymer dissolved liquid crystal composites. J Appl Phys 97:053508View ArticleGoogle Scholar
- Baldycheva A, Tolmachev VA, Berwick K, Perova TS (2012) Multi-channel Si-liquid crystal filter with fine tuning capability of individual channels for compensation of fabrication tolerances. Nanoscale Res Lett 7:387View ArticleGoogle Scholar
- Zheng WJ, Fei GT, Wang B, Zhang LD (2009) Modulation of transmission spectra of anodized alumina membrane distributed Bragg reflector by controlling anodization temperature. Nanoscale Res Lett 4:665View ArticleGoogle Scholar
- Kalachyova V, Lyutakov O, Slepicka P, Elashnikov R, Svorcik V (2014) Preparation of periodic surface structures ondoped poly(methyl metacrylate) films by irradiation with KrF excimer laser. Nanoscale Res Lett 9:951View ArticleGoogle Scholar
- Ishiguro M, Sato D, Shishido A, Ikeda T (2007) Bragg-type polarization gratings formed in thick polymer films containing azobenzene and tolane moieties. Langmuir 23:332View ArticleGoogle Scholar
- Luo S, Chen K, Cao L, Liu G, He Q, Jin G, Zeng D, Chen Y (2005) Photochromic diarylethene for rewritable holographic data storage. Optics Express 13:3123View ArticleGoogle Scholar
- Kutuvantavida Y, Williams GVM, Bhuiyan MDH (2014) Electrically modulated diffraction gratings in organic chromophore thin films. Applied Optics 53:268View ArticleGoogle Scholar
- Williams GVM, Dotzler C, Edgar A, Raymond SG (2007) Ultraviolet induced absorption and Bragg grating inscription in RbCdF3:Mn2+. J Appl Phys 102:113106View ArticleGoogle Scholar
- Williams GVM, Do MTT, Raymond SG, Ashraf M, Bhuiyan MDH, Kay AJ (2015) Optically switchable diffraction grating in a photochromic/polymer thin film. Applied Optics 54:6882View ArticleGoogle Scholar
- Natansohn A, Xie S, Richon P (1992) Azo polymers for reversible optical storage. 2. Poly[4′-[[2-(acryloyloxy)ethyl]ethylamino]-2-chloro-4-nitroazobenzene]. Macromolecules 25:5531View ArticleGoogle Scholar
- Cembran A, Bernardi F, Garavelli M, Gagliardi L, Orlandi G (2004) On the mechanism of the cis−trans isomerization in the lowest electronic states of azobenzene: S0, S1, and T1. J Am Chem Soc 126:3234View ArticleGoogle Scholar
- Wu KC, Trozzio AM (1979) Production of singlet molecular oxygen from the oxygen quenching of the lowest excited singlet state of aromatic molecules in n-hexane solution. J Phys Chem 83:3180View ArticleGoogle Scholar
- Gupta G, Steier WH, Liao Y, Luo J, Dalton LR, Jen AKY (2008) Modeling photobleaching of optical chromophores: light-intensity effects in precise trimming of integrated polymer devices. J Phys Chem C 112:8051View ArticleGoogle Scholar
- Williams GVM, Kutuvantavida Y, Janssens S, Raymond SG, Do MTT, Bhuiyan MDH, Quilty JW, Denton N, Kay AJ (2011) The effects of excited state lifetime, optical intensity, and excited state quenchers on the photostability of zwitterionic chromophores. J Appl Phys 110:083524View ArticleGoogle Scholar
- Raymond SG, Williams GVM, Do MTT, Janssens S, Lochocki B, Bhuiyan MDH, Kay AJ (2009) Photoluminescence and optical studies of photodegradation in nonlinear optical organic chromophores. Proc SPIE 7354:735408View ArticleGoogle Scholar
- Dalton LR (2003) Rational design of organic electro-optic materials. J Phys: Condens Matter 15:R897Google Scholar
- DeRosa ME, He M, Cites JS, Garner SM, Tang YR (2004) Photostability of high μβ electro-optic chromophores at 1550 nm. J Phys Chem B 108:8725View ArticleGoogle Scholar
- Magnusson R, Gaylord TK (1978) Diffraction regimes of transmission gratings. J Opt Soc Am 68:809View ArticleGoogle Scholar